The International Journal Of Engineering And Science (IJES)||Volume||2 ||Issue|| 5 ||Pages|| 01-15||2013||ISSN(e): 2319 – 1813 ISSN(p): 2319 – 1805www.theijes.com The IJES Page 1Effects of Cryogenic Treatment, Hardening and MultipleTempering On Wear Behavior of D6 Tool Steel1,R.H.Naravade, 2S.B.Belkar , 3,R.R.Kharde1.Lecturer,Department of Mechanical Engineering, P.Dr.V.V.P.Polytechnic,Loni2,Assistant Professor, Department of Mechanical Engineering, P.R.E.C.,Loni3,Head,Department of Mechanical Engineering, P.R.E.C.,Loni--------------------------------------------------------ABSTRACT-------------------------------------------------------------This experimental work intended to investigate the effects of cryogenic treatment on the wear behavior ofD6 tool steel. For this purpose, the temperature was used -185oC as deep cryogenic temperature. The effectsof cryogenic temperature (deep), cryogenic time (kept at cryogenic temperature for 36 hr) on the wearbehavior of D6 tool steel were studied. The findings showed that the cryogenic treatment decreases theretained austenite and hence improves the wear resistance and hardness. Due to more homogenized carbidedistribution as well as the elimination of the retained austenite, the deep cryogenic treatment demonstratedmore improvement in wear resistance and hardness compared with the conventional heat-treatment. Byincreasing the keeping time at cryogenic temperatures, more retained austenite was transformed intomartensite; thus, the wear resistance was improved and further hardness were observed.This experimentalwork also intended to investigate the role of multiple tempering before and after cryogenic treatment onfriction and wear behaviour of D6 tool steel as classified by American Iron and Steel Institute (AISI). D6 toolsteel is used for measuring tools, blanking dies, forming dies, coining dies, long punches, forming rolls,edging rolls, master tools, extrusion dies, drawing dies, moulds for pressing abrasive powders etc.Thedifferent combination of heat treatments like hardening (at 1020°C) for one hour, tempering (at 210°C) fortwo hours and deep cryogenic treatment (at -185°C) for 36 hours was done on D6 tool steel. Wear test wereperformed using pin-on-disc wear tester to which two different normal loads (3.1Kg and 5.1Kg) and twodifferent velocities (1.5m/s and 2.5m/s) were applied. Hardness of specimens was measured by using RockwellHardness tester. Microstructural characterizations of the differently heat treated specimens have been done byimage analyzer software with inverted microscope.The findings show that the cryogenic treatment improvesthe wear resistance and hardness of D6 tool steel. The results indicate that, in HCT specimens there was largereduction in the wear rate and markedly enhancement in wear resistance of the D6 tool steel.KEYWORDS: - AISI D6 tool steel, cryogenic treatment, wear rate and wear resistance.-------------------------------------------------------------------------------------------------------------------------------------Date of Submission: 17thMay 2013, Date of Publication: 05thJune 2013-------------------------------------------------------------------------------------------------------------------------------------I. INTRODUCTIONTo understand the effects of cryogenic processing it is essential that one can be acquainted with theheat treating of metals. The primary reason for heat treating steel is to improve its wear resistance throughhardening. Gears, bearings, and tooling for example are hardened because they need excellent wear resistancefor extended reliability and performance .Cryogenic processing (CP) is presently employed in the fields like aerospace and manufacturingindustries, sports and music instruments, firearms etc. for performance enhancement of various components. Inthe last decade, a good number of investigations have been directed to improve the tribological properties likewear resistance of tool/die steels by cryotreatment. Cryogenic treatment of tooling steels is a proven technologyto increase wear resistance and extend intervals between component replacements for dies, punches, drill bits,end mill cutters, bearings, cams, crankshafts, blocks, pistons, blades etc. Controlled CP is commonly appendedin-between conventional hardening and tempering treatments for tool/die steels . The execution of the deepcryogenic treatment on quenched and tempered high speed steel tools increases hardness, reduces tool
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 2consumption and down time for the equipment set up, thus leading to cost reductions of about 50% .In lastfew years it is found that the use of combination of different heat treatment like hardening, multiple temperingand cryogenic treatments affect on the friction and wear behaviour of AISI D6 tool steel .II. AISI D6 TOOL STEELTool steels were developed to resist wear at temperatures of forming and cutting applications. Toolsteel is used on a wide variety of applications where resistance to wear, strength, toughness and otherproperties are selected for optimum performance. They are broadly divided into six categories: cold work,shock resisting, hot work, high speed, mold and special-purpose tool steels .Generally speaking, many toolsteels fulfill the requirements for a given application, so that final selection is guided by considering the toollife as well as the cost of material and fabrication. First reasonable factor affecting the tool life is adhesionwear . The high-carbon, high-chromium cold work tool steel, designated as group D (Deep Hardening) steelin the AISI classification system, are the most highly alloyed cold-work steel. The high-carbon, high-chromium cold work D6 tool steel has extremely high wear and abrasion resistance. Again, the high alloycontent provides excellent hardenability and good dimensional stability. D6 tool steel contributesapproximately 21% of total tool steel application. Although the high abrasion resistance of the D6 tool steels isdesirable for cold-work applications, the machining and grinding operations during manufacturing of finisheddies and molds are difficult.A. Applications of D6 Tool SteelMeasuring tools, blanking dies, forming dies, coining dies, slitting cutters, heading tools, longpunches, forming rolls, edging rolls, master tools, beading rolls, intricate punches, extrusion dies, drawingdies, lamination dies, thread rolling dies, shear blades, burnishing tools, gauges, knurls, wear parts, plasticmoulds, decorative knives, hunting knives, mill rolls, spinning tools, moulds for pressing abrasive powders etc.III. LITERATURE REVIEWIn tool steels, a low percentage of austenite is retained after the conventional heat-treatment named„„retained austenite”. The retained austenite as a soft phase in steels could reduce the product life and, inworking conditions, it can be transformed into martensite. This new martensite could cause several problemsfor working tools. This new martensite is very brittle and differs from the tempered one, which is used in tools.Furthermore, this martensite causes micro cracks and reduces the product life. Moreover, the retainedaustenite-to-martensite transformation provides dimensional instability.Regarding the problems mentioned above, the controlled transformation of the retained austenite intomartensite is essential to many types of component. In order that this transformation occurs, the cryogenictreatment is used. As a result, the retained austenite is reduced and higher wear resistance is obtained. Twotypes of cryogenic treatment are usually applied as follows: (1) the shallow cryogenic treatment (SCT) isperformed between -50oC and -100 oC after quenching. In SCT, the retained austenite is reduced and higherwear resistance is obtained in tool steels; (2) the deep cryogenic treatment (DCT) is conducted at thetemperatures below -125oC. This treatment reduces or eliminates the retained austenite and distributes carbidesin a higher proportion and in a more homogenized manner. Accordingly, further wear resistance as comparedwith SCT was observed. At DCT temperatures, austenite and martensite lattice is contracted. As a result of thiscontraction, carbon atoms are forced to diffuse. At higher temperatures, these carbon atoms would produce thenew carbides, thereby leading to more homogenized carbide distribution [1-10].A. Akhbarizadeh et.al  studied the effects of cryogenic treatment on the wear behavior of D6 toolsteel. For this purpose, two temperatures were used: -63ºC as shallow cryogenic temperature and -185ºC asdeep cryogenic temperature. The effects of cryogenic temperature (Shallow and deep), cryogenic time (kept atcryogenic temperature for 20 hours and 40 hours) and stabilization (kept at room temperature for one week) onthe wear behavior of D6 tool steel were studied. Wear tests were performed using a pin-on-disk wear tester.Due to more homogenized carbide distribution as well as the elimination of the retained austenite, the deepcryogenic treatment demonstrated more improvement in wear resistance and hardness compared with theshallow cryogenic treatment. By keeping the samples for a period of one week at room temperature afterquenching (stabilization), more retained austenite was transformed into martensite and higher wear resistanceand higher hardness were achieved.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 3B. Summary of Literature ReviewRecent studies have indicated that cryogenic treatment is an essential supplementary treatment,which is performed on products after conventional heat-treatment in order to increase their wear resistance insome materials and to produce dimensional stability in others. The cryogenic treatment is conducted on toolsteels, maraging steel, cast iron, carburized steel, tungsten carbide, polymers and composites. In all of thematerials mentioned, the cryogenic treatment increases the wear resistance and subsequently increases theproduct life. The cryogenic treatment has been used as a finishing process in the past few decades. This processis also being used in aircraft and automobile industries as well as many other areas.Over the last decade,several researchers [1–10] have reported that the Deep Cryogenic Treatment (DCT) considerably improves thewear resistance (WR) of AISI D6 tool steels than those obtained either by Cold Treatment (CT) or byConventional Heat Treatment (CHT). Also it is found that the considerable reduction in wear rate (WR) andcoefficient of friction (µ).In addition, it has also been reported that DCT and multiple tempering aftercryogenic treatment enhances the dimensional stability and reduces the residual stresses. These favourableeffects increase the service life of the components made of AISI D6 tool steels.Literature of past work does not adequately clarify the selection of tempering, cryogenic temperatureand soaking time. There is a need to standardize the process for cryogenic treatment in particular tool steelsand understand the underlying metallurgical mechanism responsible for improvement of wear. In generalcryogenic treatment and multiple tempering is still in the dormant level as far as wear rate, wear resistance andcoefficient of friction is concerned. This is the main focus of the present work on D6 tool steel.C. Problem DefinitionEffects of cryogenic treatment on wear behavior of D6 tool steel and effect of multiple temperingbefore and after the cryogenic treatment.D. ObjectivesTherefore the present investigation is based on the effect of cryogenic treatment on friction and wearbehaviour of AISI D6 tool steel and has following objectives,1) To study the effect of wear test parameters like normal load, velocity of counter disc on friction andwear behaviour of D6 tool steel.2) To study the effect of different heat treatments like hardening, cryogenic treatment and multipletempering on wear volume, coefficient of friction, wear rate and wear resistance of D6 tool steel.3) To study the relationship between normal loads, velocity of counter disc, coefficient of friction, wearrate and wear resistance.4) To find percentage improvement in wear resistance due to combination of different heat treatments onD6 tool steel.5) It is intended that, this research will be useful in promoting the applications of cryogenic treatment onD6 tool steel.E. Proposed Experimental WorkFor improvement of friction and wear behaviour of AISI D6 tool steel, combination of different heattreatments like hardening, multiple tempering, cryogenic treatments are used. In this study hardeningtemperature 1020°C for one hour, tempering temperature 210°C for two hours, cryogenic temperature -185°Cfor 36 hours, soft tempering temperature 100°C for one hour were selected. The reduction in wear rate,coefficient of friction; improvement in wear resistance of specimens were assessed by a pin-on-disk weartesting machine. For wear test the disc are made of EN-35 (68 HRC maintained) of surface roughness, Ra =0.5 μm. Testing conditions were used as follows,a. Normal Load, FN = 3.1Kg, 5.1Kgb. Sliding speed, V = 1.5, 2.5 m/sc. Test Duration, T = 60 Min.Change in hardness of specimens was measurement by using Rockwell Hardness tester.Microstructural characterizations of the differently heat treated specimens have been done by image analyzersoftware with inverted microscope.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 4IV. EXPERIMENTAL DETAILSTo ensure a high-quality product, diagrams and lettering MUST be either computer-drafted or drawnusing India ink.a. MaterialThe present investigation has been conducted with samples of AISI D6 tool steel. AISI D6 tool steel isalso designated as T30405 by Unified Numbering System. The round bars of diameter 9.20mm were selectedfor this experimentation. The specimens for wear test were prepared of diameter 9.20mm and height 30mm.For hardness test specimens were prepared of diameter 9.20mm and height 10mm. The chemical compositionof specimens has analyzed by Optical Emission Spectrometer (ASTM-E-1066-2008). Table no. 4.1 conforms tothe chemical composition of AISI D6 tool steel.Table no. 4.1 Chemical Composition of D6 Tool SteelSr. No. ElementWeight PercentageActual%AISI Specification of D6 ToolSteel1 C 2.16 2.00-2.352 Mn 0.38 0.60 Max.3 Si 0.35 0.30-0.504 S 0.011 0.030 Max.5 P 0.015 0.030 Max.6 Cr 12.02 11.00-13.007 Mo Nil --8 W 0.23 1.00 Max.b. TreatmentsThe material selected for this work was given various treatments and treatment combinationsindicated in Table no. 126.96.36.199.HardeningThe first step in the heat treatment of AISI D6 tool steel was hardening. The purpose of hardeningwas to harden steel to increase the wear resistance, cutting ability. Hardening of AISI D6 tool steel was done inthe tubular furnace (3.5KW, 230V AC, 15A, 1200±10°C) at a temperature of 1020°C [1, 6] for 1 Hour. Duringhardening process, inert gas Argon was supplied in tubular furnace to avoid oxidation. Harden AISI D6 toolsteel followed air cooling which provides great benefit of minimizing distortion and dimensional changes .Table no. 4.2 Different Heat Treatments Employed to AISI D6 tool steelSr.No. Nomenclature Particulars of Treatment1 HT Hardening (1020°C for 1 Hr), Single Tempering (210°C for 2 Hr)2 HTT Hardening (1020°C for 1 Hr), Double Tempering (210°C for 2 Hr)3 HTTT Hardening (1020°C for 1 Hr), Triple Tempering (210°C for 2 Hr)4 HCTHardening (1020°C for 1 Hr), Cryotreated (-185°C for 36 Hr), SingleTempering (210°C for 2 Hr)5 HCTTHardening (1020°C for 1 Hr), Cryotreated (-185°C for 36 Hr), DoubleTempering (210°C for 2 Hr)6 HCTTTHardening (1020°C for 1 Hr), Cryotreated (-185°C for 36 Hr), TripleTempering (210°C for 2 Hr)7 HCSTHardening (1020°C for 1 Hr), Cryotreated (-185°C for 36 Hr), SoftTempering (100°C for 1 Hr)8 HTCSTHardening (1020°C for 1 Hr), Single Tempering (210°C for 2 Hr),Cryotreated (-185°C for 36 Hr), Soft Tempering (100°C for 1 Hr)9 HTTCSTHardening (1020°C for 1 Hr), Double Tempering (210°C for 2Hr),Cryotreated (-185°C for 36 Hr), Soft Tempering (100°C for 1Hr)10 HTTTCSTHardening (1020°C for 1 Hr), Triple Tempering (210°C for 2 Hr),Cryotreated (-185°C for 36 Hr), Soft Tempering (100°C for 1 Hr)
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 54.2.TemperingThe process which consists of heating the hardened components to a temperature between 100°C and700°C, holding at this temperature for specific period and cooling to room temperature, usually by air is calledas „tempering‟.The purposes of tempering are as follows,a. To relieve the internal stresses developed due to rapid cooling of steels after hardening process and due tovolume changes occurring in the austenite to martensite transformation, to reduce brittleness,b. To reduce hardness and to increase ductility and toughness,c. To eliminate retained austenite .Tempering of D6 tool steel was done in the muffle furnace (3.8KW, 230V AC, 600±10°C). Samplesof treatment HT, HTT, HTTT, HCT, HCTT, HCTTT, HTC, HTTC and HTTTC after H and HC wereimmediately subjected to tempering at temperature of 210°C with 2 Hr soaking time, followed by air cooling toroom temperature, that is, single tempering. After the air cooling the remaining samples were subjected todouble tempering for the same temperature and time and then air cooled. Similar procedure is again followedfor triple tempering on the remaining samples from double tempering. The detailed heat treatments areindicated in Table no. 188.8.131.52.Cryogenic TreatmentThe cryogenic treatment was done in Cryoprocessor system at Nashik Cryogenic Services,Nashik.Fig.4.1 Cryoprocessor SetupCryoprocessor is capable of maintaining shallow subzero treatment, deep subzero treatment andcryogenic subzero treatment temperatures for any length of time through software based program whichcontrol the flow of liquid nitrogen via solenoid valve as per the demand of programming logic controller. Thearrangement of cryoprocessor is as shown in Fig. 4.1. As soon as liquid nitrogen enters into Cryoprocessor, itgasifies immediately through multi hole slitter and thus cooling of the specimen takes place. Temperature ofthe bath is sensed using Resistance Temperature Detector, which provides online feedback of temperature ofthe bath to regulate the flow of liquid nitrogen.Fig. 4.2 Block Diagram of Cryoprocessor
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 6Schematic line diagram of Cryoprocessor used in this experiment is as shown in Fig. 4.2. In thepresent work, the specimens were cryotreated at -185°C, the soaking time was selected 36 Hr . The bath wasallowed to cool down slowly (3- 4°C/ min) to avoid thermal shocks.Once the subzero treatment was over, allthe specimens were allowed to warm up in an insulated thermocol box which takes normally 16-24 hr to reachthe room temperature depending on the treatment given. A computer generated thermal profile of the processoris shown in Fig. 4.3. Blue line stands for instantaneous process temperature and red line stands for set pointwhich was maintained manually. It must be noted that the actual process temperature follows the set points.After cryogenic treatment the specimen of HTCST, HTTCST, HTTTCST and HCST are followed bysoft tempering. Soft tempering was done in muffle furnace (3.8KW, 230V AC, 600±10°C) at 100°C for oneHr.Fig. 3.3 Computer Generated Thermal Profile of Cryoprocessorc. MetalographyMicrostructure analysis was carried by image analyzer software; with inverted microscope (Make-CARL ZEISS Germany, Model-Axiovert 40Mat). Carefully prepared samples were first surface leveled onendless emery belt (80/0) paper. Further samples were subjected to separately polishing on emery paper (240,400, 600, 800 and 1000) so as to make surface free from scratches. Final polishing was done on velvet clothpolishing machine with intermittent application of fine suspensions of alumina to get better finish on polishedsurface. A freshly prepared etchant „‟ Nital‟‟, of composition approximately 5 ml Nitric acid with 100 ml ethylalcohol (i.e. approximately 5%), was used for revealing micro constituents of AISI D6 tool steel.Microstructures were then recorded by image analyzer system as shown in Fig. 4.4. Chromium carbides aredivided in two categories viz. small size carbides, maximum dimension less than 1 micron, and big carbides,any larger dimension more than 1 micron.(a) (b) (c)
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 7(d) (e) (f)(g) (h) (i)(j)Fig. 4.4 Microstructure of AISI D6 tool steel for different heat treatments samples at 1000x: a) HT, b)HTT, c) HTTT, d) HCT, e) HCTT, f) HCTTT, g) HC, h) HTC, i) HTTC, j) HTTTCd. Hardness MeasurementThe hardness of polished AISI D6 tool steel specimens was measured on a Rockwell hardness testingmachine. The samples prepared for metallography, are used for hardness measurement. The hardness ismeasured on “C” scale with 10Kg minor load and 150Kg major load applied. A minimum of 5 readings havebeen taken to estimate the average value of hardness of the specimen. The hardness of different samples isshown in Table no. 4.3.Table no. 4.3 Hardness of SpecimensSr. No. Sample Hardness (HRC) Hardness (VHN)1 HT 59.8 6932 HTT 60.4 7073 HTTT 60.6 7124 HCT 62.8 7705 HCTT 62.2 7536 HCTTT 61.4 7327 HCST 60.1 7008 HTCST 60.7 7159 HTTCST 60.3 70510 HTTTCST 60.1 700
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 8e. Evaluation of Wear BehaviourIn order to investigate the resistance of the heat treated AISI D6 tool steels to adhesion wear; thecomputerized pin-on-disc tribometer as shown in Fig. 4.5 was used. Dry sliding wear tests were carried out onthis computerized pin-on-disc wear testing machine (DUCOM: TR 20LE, India). The specifications of pin-on-disc tribometer are shown in Table no. 4.5. Specimens of 9.20mm diameter and 30mm length was clamped ina holder and held against the rotating counter disc made of WC-coated EN-35 (68 HRC) with the roughnessvalue, Ra = 0.5µm. The faces of the pin specimens were polished and cleaned in acetone in an ultrasoniccleaner. The wear tests were carried out at two different normal loads (FN) of 30.41N (3.1 Kg) and 50.03N (5.1Kg) at a constant linear sliding velocity (V) of 1.5m/s and 2.5m/s in dry condition at the room temperature.The values estimated nominal contact pressure in the pin specimens are 0.4575MPa and 0.7526MPacorresponding to FN of 3.1Kg and 5.1Kg respectively. The wear tests were carried for 60 minutes duration. Allthese values are shown in Table no. 4.4. The surface of each specimen was cleaned at each time before eachtest. Every time new track radius of rotating disc was used so that pin was exposed to fresh surface of counterface. Wear and frictional force was measured continuously through a load cell measuring the tangential force.Fig. 4.5 Experimental Setup of Pin-on-disc TribometerWear rates (WR) have been estimated by volumetric method from the recorded cumulative height loss ofthe specimens with respect to sliding distance in the steady-state wear regime considering mean of at least twotest results under identical conditions.Table no. 4.4 Wear Test DetailsSr. No. Normal Load FN (Kg, N) Pressure P (MPa) Velocity V (m/s)1 3.1,30.41 0.4575MPa 1.52 3.1,30.41 0.4575MPa 2.53 5.1,50.03 0.7526 MPa 1.54 5.1,50.03 0.7526 MPa 2.5Table no. 4.5 Specifications of pin on disc Tribometer (TR-20)Make Ducom Ltd, Bangalore.Pin Size 3 to 12 mm diagonalDisc Size 160 mm dia. X 8 mm thickWear Track Diameter (Mean) 10 mm to 140 mmSliding Speed Range 0.26 m/sec. to 10 m/sec.Disc Rotation Speed 100-2000 RPMNormal Load 200 N MaximumFriction Force 0-200 N, digital readout, recorder outputWear Measurement Range 4 mm, digital readout, and recorder outputPower 230 V, 15A, 1 Phase, 50 Hz
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 9Table no. 4.6 Rotating Disc Speed in rpmSr.No.Sliding Velocity DiscV(m/s)Wear Track DiameterD(m)Disc SpeedN(rpm)11.50.060 477.52 0.080 358.13 0.100 286.54 0.116 246.952.50.060 795.86 0.080 596.87 0.100 477.58 0.116 411.6V. RESULTS AND DISCUSSIONa. Microstructure EvaluationMicrostructure of D6 tool steel for HT, HTT, HTTT, HCST, HTCST, HTTCST and HTTTCSTspecimens exhibit non-uniform distribution of large, elongated, white regions of primary chromium carbidesand uniform distribution of nearly spherical secondary chromium carbides. But for HCT, HCTT and HCTTTspecimens there is uniform distribution of white regions of primary chromium carbides and nearly sphericalsecondary chromium carbides. It is clearly seen that there is definite reduction in carbide size as seen in Fig.5.4 (d) as compared to original structure as seen in Fig. 5.4 (a).b. Hardness StudyFig. 5.1 Hardness test report of D6 tool steel for different heat treatmentThe measured Rockwell hardness number of D6 tool steel for different heat treatments is tabulated inTable no. 5.3. The results show that the cryogenic treatment increases hardness. From Fig. 5.1, it is observedthat for D6 tool steel the hardness of HCT specimens improves approximately 5% as compared to HTspecimens. It is also observed that the hardness value for multiple tempering before and after cryotreatmentwere decreases. The hardness values for specimens subjected to different heat treatment can be directly relatedto the magnitude of reduction of soft retained austenite with associated improvement in the amount of hardsecondary carbides and tough tempered martensite . The obtained results thus infer that increase in hardnessof D6 tool steel specimens occurs due to cryotreatment.c. Wear Mechanismi.Wear VolumeThe wear volumes of the D6 tool steel versus sliding time are presented in Fig. 5.2 - 5.5 for differentwear test parameters. It is observed that both normal load and sliding velocity affect the wear volume, which
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 10attains values between 1.596 mm3to 11.365 mm3. The wear volume increases with increasing normal load, butwear volume of the D6 tool steel observed to be fluctuating with increase in sliding speed.It was observed that the cryogenically treated specimens have less wear as compared to conventionalheat treatment specimens. Apparently there is no straight correlation with hardness. Even though difference ofhardness of HT and HCT specimens is not much more, there is a dramatic drop in wear volume in wear test.There is an increasing wear volume reflected in multiple tempering specimens. From wear test report it isobserved that the wear volume was increased in the order of HCT, HCTT, HCTTT, HCST, HTCST, HTTCST,HTTTCST, HTTT, HTT and HT specimens. In the case of HCT Specimens, the large reduction in wear couldbe mainly due to the retained austenite elimination and the homogenized carbide distribution as well as morechromium carbide as compared to other heat treated specimens.Fig. 5.2 Wear of D6 tool steel for 3.1Kg load and Fig. 5.3 Wear of D6 tool steel for 3.1Kload and1.5m/s Velocity for different heat treatment 2.5m/s velocity for different heat treatmentFig. 5.4 Wear of D6 tool steel for 5.1Kg load and Fig.5.5 Wear of D6 tool steel for 5.1Kg load and1.5m/s velocity for different heat treatment 2.5m/s velocity for different heat treatment5.1. Coefficient Of FrictionThe coefficient of friction of D6 tool steel for the different wear conditions for tests carried out and itis observed that, the value of coefficient of friction varies approximately from 0.5324 to 0.7449. Thecomparison of coefficient of friction between different heat treated specimens is as shown in Fig. 5.6 - 5.9. It isobserved that the coefficient of friction decreases with increase in normal load. Wear test report reflect that thecoefficient of friction of D6 tool steel increases due to multiple tempering before and after the cryogenictreatment. For HCT specimens the value of coefficient of friction is very less due to largest hardness ascompared to other type of specimens. The coefficient of friction of D6 tool steel observed to be fluctuating withincrease in sliding speed.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 11Fig. 5.6 Coefficient of Friction of D6 tool steel for Fig. 5.7 Coefficient of Friction of D6 tool steel for3.1Kg load and 1.5m/s velocity for different heat 3.1Kg load and 2.5m/s velocity for different heattreatment treatmentFig. 5.8 Coefficient of Friction of D6 tool steel for Fig. 5.9 Coefficient of Friction of D6 tool steel for5.1Kg load and 1.5m/s velocity for different heat 5.1Kg load and 2.5m/s velocity for different heattreatment treatment5.2. Wear Rate (Wr)The computed values of wear rate for all type of D6 tool steel for specimens tested under normal loads3.1Kg and 5.1Kg are as shown in Fig. 5.10 - 5.13. It is observed that both normal load and sliding velocityaffect the wear rate, which attains values between 0.2955 mm3/m to 1.9942 mm3/m. The results in thesefigures show that the wear rate of HCT specimens is very less as compared to other type of heat treated samplesand where as there is an increasing wear rate reflected in double and triple tempered D6 tool steel. In the caseof HCT specimens, the large reduction in wear rate could be mainly due to the homogenized carbidedistribution, additional amount of fine carbides nucleated during cryogenic treatment and reduction in carbidesize as compared to other heat treated specimen‟s i.e.Wear behavior is highly influenced by microstructural parameter like carbide size and its distribution.It is also observed that the wear rate increase linearly with increasing normal load for all types of specimens.High wear rate in case of HT, HTT, HTTT, HCTT, HCTTT, HCST, HTCST, HTTCST, and HTTTCSTspecimens as compared to HCT specimens could be attributed to primary coarse carbides. The lowest wear rateis shown by HCT specimens as a result of additional amount of the fine carbides nucleated during cryogenictreatment.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 12Fig. 5.10 Wear Rate of D6 tool steel for 3.1Kg load Fig. 5.11 Wear Rate of D6 tool steel for 3.1Kgload and 1.5m/s velocity for different heat treatment and 2.5m/s velocity for different heat treatmentFig. 5.12 Wear Rate of D6 tool steel for 5.1Kg load Fig. 5.13 Wear Rate of D6 tool steel for 5.1Kg loadand 1.5m/s velocity for different heat treatment and 2.5m/s velocity for different heat treatment5.3.Wear Resistance (Wr)Wear behavior can be conveniently expressed in terms of dimensionless wear coefficient (k). Theinverse of dimensionless wear coefficient is known as wear resistance (WR). The calculated wear resistance ofdifferent heat treated specimens are as shown in Fig. 5.14 - 5.17. The results obtained in this study, in general,are in agreement with results reported by Dass et al . In this study it is observed that the improvement inwear resistance is significant by cryogenic treatment.5.4.Improvement in wear resistance (α %)In order to quantify the magnitude of improvement of WR by HCT over that of HT treatmentspecimens, a parameter has been considered here, which is defined as follows,α % = [ ] × 100Where, WR is wear resistance, HCT and HT denote the type of the specimen [5, 7].The value of havebeen calculated for different types of specimens under different test conditions. As compared to other type ofsamples, there is greatest improvement in wear resistance in case of HCT samples. The results shown that for3.1 kg and 5.1Kg normal load, at 1.5m/s and at 2.5m/s velocity, which illustrates that in comparison to HT,HCT treatment enhance the WR of D6 tool steel by 140.501% to 248.559%. In addition, the magnitude of forHT and HCT specimens decreases with the increasing normal load and velocity.The relation between wear properties with the results of microstructure analysis revels that theimprovement in wear resistance is depends on the microstructure analysis generated by different heattreatments irrespective of its dependence on wear test conditions. It can be concluded at this stage that thereduction of retained austenite content, reduction in size of the secondary carbide and distribution of secondarycarbides are basic factors responsible for the improvement in wear resistance in HCT specimens; whereas wearresistance property deteriorates with double and triple tempering as evident from Fig. 5.14 - 5.17. In the HT,
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 13HTT, HTTT, HCTT, HCTTT, HCST, HTCST, HTTCST, and HTTTCST of D6 tool steel specimens there isgrowth in secondary carbide size. This contributes in deteriorating the wear resistance of D6 tool steel.This experimental work shows that the combined effect of heat treatment and cryogenic treatment can assist inimproving wear resistance in single tempering, whereas wear resistance deteriorate in subsequent double andtriple tempering.Fig. 5.14 Wear Resistance of D6 tool steel for 3.1Kg Fig. 5.15 Wear Resistance of D6 tool steel forload and 1.5m/s velocity for different heat treatment 3.1Kg load and 2.5m/s velocity for different heattreatmentFig. 5.16 Wear Resistance of D6 tool steel for 5.1Kg Fig. 5.17 Wear Resistance of D6 tool steel for 5.1Kgload and and 1.5m/s velocity for different heat load 2.5m/s velocity for different heat treatmenttreatmentd. Statistical Regression AnalysisStatistical regression analysis is the study of the relationship between two or more variables, used toestablish the empirical equation relating input-output parameters, by utilizing least square method. Moreover,it is the most commonly used statistical modeling technique developed based on experimental data. There isdifference between predicated and actual values of the response for the same set of independent variables. It ispossible to attribute this difference to a set of independent variable and the difference due to random orexperimental errors. The technique of analysis of variance (ANOVA) does this. With the help of regressioncoefficients we can calculate the correlation coefficients. The square of coefficients, called coefficients ofdetermination R2(R-Sq), measures the degree of association of correlation that exists between the variables.The value of R2(R-Sq) is the important criteria to decide the validity of regression model. In general, greaterthe value of R2(R-Sq) better is the fit and more useful the regression equation is as predictive device. If value is0.85(85%) or more, then relationship established by regression model is acceptable.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 145.5. Regression Analysis for D6 Tool Steel SpecimensThe regression analysis was done on Minitab 16 Software for Wear Rate versus Load, Speed andfollowing regression equations has been developed to predict the wear rate for HCT specimen.Regression Analysis: Wear Rate versus Load, SpeedThe regression equation isWear Rate = - 0.000449 + 0.000191 Load + 0.000111 SpeedPredictor Coef SE Coef T PConstant -0.00044934 0.00007108 -6.32 0.100Load 0.00019063 0.00001222 15.59 0.041Speed 0.00011075 0.00002445 4.53 0.138S = 0.00002445 R-Sq = 99.9% R-Sq(adj) = 99.6%Analysis of VarianceSource DF SS MS F PRegression 2 1.57617E-07 7.88086E-08 131.83 0.061Residual Error 1 5.97802E-10 5.97802E-10Total 3 1.58215E-07Source DF Seq SSLoad 1 1.45352E-07Speed 1 1.22656E-08It was observed that the regression analysis carried out shows that, the value of R2(R-Sq) for HCTspecimen has greater the value 99.6%, thus better is the fit and more useful the regression equation is aspredictive device.VI. CONCLUSIONThe present investigation is based on the effect of cryogenic treatment on friction and wear behaviour ofAISI D6 tool steel. After conducting the experimental work, following conclusions are drawn from the results.1) The wear volume and wear rate (WR) increases linearly with increasing normal load for all type ofsamples, whereas coefficient of friction decreases with increase in normal load.2) It is observed that at higher velocities, wear rate is enhanced, but the coefficient of friction observed tobe fluctuating.3) It is seen that the largest improvement in wear resistance (WR) is observed in HCT specimens, which is140% to 248% that of the HT specimens. Subsequent tempering, i.e. double and triple temperingdeteriorates wear resistance. The improvement in WR decreases with increasing severity of wear testconditions, i.e. increasing normal load.4) Wear volume, coefficient of friction, wear rate and wear resistance of the materials depends upon thecombination of heat treatments.5) The Rockwell hardness number of HCT specimens improves approximately 5% by HT specimens.Cryogenically treated specimen shows decreasing hardness from single stage to triple stage tempering.6) Therefore, among different heat treatments like HT, HTT, HTTT, HCT, HCTT, HCTTT, HCST,HTCST, HTTCST and HTTTCST; the lowest wear volume, coefficient of friction and wear rate isobserved in HCT specimens.As a result of the lower retained austenite, the cryogenic treatment improves the wear resistance andthe hardness of the D6 tool steel. This improvement is significant in the deep cryogenic treatment due to morehomogenized carbide distribution, the retained austenite elimination and higher chromium carbide percentagein comparison with the conventional heat treatments.
Effects Of Cryogenic Treatment, Hardening…www.theijes.com The IJES Page 15REFERENCESJournal Papers: L. Bourithis, G.D. Papadimitriou, J. Sideris; “Comparison of wear properties of tool steels AISI D2 and O1 with the same hardness”;Tribology International 39 (2006), pp 479-489. M. H. Staia, Y. Perez-Delgado, C. Sanchez, A. Castro, E. Le Bourhis, E.S. Puchi-Cabrera; “Hardness properties and high-temperaturewear behavior of nitrided AISI D2 tool steel, prior and after PAPVD coating”; Wear 267 (2009), pp 1452-1461. A. Molinari, M. Pellizzari, S. Gialanella, G. Staffelini, K. H. Stiansy; “Effect of deep cryogenic treatment on the mechanical propertiesof tool steels”; Journal of Materials Processing Technology 118 (2001), pp 350-355. N. B. Dhokey, S. Nirbhavne; “Dry sliding wear of cryotreated multiple tempered D-3 tool steel”; Materials Processing Technology 209(2009), pp 1484-1490. D. Das, A.K. Dutta, K.K. Ray; “Correlation of microstructure with wear behavior of deep cryogenically treated AISI D2 steel”, Wear267 (2009), pp 1371-1380. Cord Henrik Surberg, Paul Stratton, Klaus Lingenhole; “The effect of some heat treatment parameters on the dimensional stability ofAISI D2”; Cryogenics 48 (2008), pp 42-47. D. Das, A.K. Dutta, K.K. Ray; “Optimization of the duration of cryogenic processing to maximize wear resistance of AISI D2 steel”;Cryogenics 49 (2009), pp 176-184. A. Akhbarizadeh, A. Shafyei, M.A. Golozar; “Effects of cryogenic treatment on wear behavior of D6 tool steel”; Materials and Design30(2009), pp 3259–3264. N. Saklakoglu, I.E. Saklakoglu, V. Ceyhun, O. R. Monteiro, I.G. Brown; “Sliding wear behaviour of Zr-ion-implanted D3 tool steel”;Tribology International 40(2007), Analysis of Friction And Wear Behaviour of D2 Tool Steel 84 pp 794–799. O. Barrau, C. Boher, R. Gras, F. Rezai-Aria; “Analysis of the friction and wear behavior of hot work tool steel for forging”; Wear 255(2003), pp 1444-1454.Books: G. Roberts, G. Krauss, R. Kennedy; “Tool Steel”, Fifth Edition, ASM International, Latrobe, Pennsylvania, 1980, pp. 1-28 & 203-218. V. D. Kodgire, S. V. Kodgire; “Material Science and Metallurgy for Engineers”, Twenty Sixth Edition, Everest Publishing House,2010, pp. 30 8-416. T. A. Stolarski., “Tribology in Machine Design”, First published 1990, Reprinted 2000, Butterworth-Heinemann, Oxford, 1994, pp.13-63.Websites: www.Tribology-abc.com/calculators/hardness.htm.Biographies and Photographs:Rahul H.Naravade, Pursuing ME Design Engineering, Lecturer in Mechanical Engineering Department inP.Dr.V.V.P.Polytechnic Loni. Prof.S.B.Belkar, ME Design,Asst.Professer in P.R.E.C. Loni. Prof.R.R.Kharde, ME Tribology,Professer & H.O.D. in Mechanical Engineering Department inP.R.E.C.Loni.